paper 30 advanced casting simulations manuscript final
Post on 12-Nov-2014
Embed Size (px)
ADVANCED CASTING SIMULATIONSMarco Aloe, Dominique Lefebvre, Alfons Mackenbrock ESI Group, France Adi Sholapurwalla, Sam Scott - ESI NA, USA
ABSTRACT Beyond simply identifying shrinkage porosity and filling problems, numerical tools have been further developed to predict stresses, microstructures, defects and to model specific processes that can be used effectively by the foundry engineer early in the manufacturing process to save significant time and cost. More specifically this paper will address the following topics: Stress and deformation - what is the final shape of the cast component? What about fatigue life of the die? Can heat transfer variation due to gap formation between the casting and the die be taken into account? Can hot tears defects be predicted? Micro and gas porosity - what about the integrity of the part? What about the initial gas content in the liquid? As-cast mechanical properties - can local mechanical properties be predicted such as yield strength and hardness? Core blowing - can core defects be simulated? The author will discuss the above subjects and will show how international research projects and industrially leaded projects are essential to improve casting simulation capacities.
KEYWORDS FEM, casting simulation, stress, deformation, gas porosity, microstructure, mechanical properties, core blowing, ProCAST, PAM-QUIKCAST.
INTRODUCTION With the generalization of CAD 3D modelling and the increase of computing performance, casting simulation software has reached a state where a relevant input for the design of a die can be given to the process engineers. Gating systems, overflows, venting channels can be optimized using numerical simulation. Solidification related defects like hot spots can also be predicted taking into account cooling channels and die cycling so as to accurately reproduce production conditions. Today, most of the casting simulation packages in the market can handle solidification and fluid flow in the casting with satisfactory accuracy. Now, the foundry industry wants to focus on more advanced predictions such as stress and deformation, microstructure determination, as-cast mechanical properties, microporosity indication and core blowing defects.
STRESS AND DEFORMATION Besides the defects related to filling and solidification, there are a number of stress related issues which can affect the final integrity of the cast component as well as result in die failure. One of the main goals of the casting process still remains to approach and achieve net shape. Indeed, large deformation or distortion in the part requires more rework, like hot pressing, even after a heat treatment operation. Factors which influence the stress behaviour and fatigue life of the die include geometry, thermal history (metal temperature, gap formation, die spraying, cooling/heating channel), material properties of the die and the casting, external forces and pressures. In order to accurately simulate the stress behaviour, one should consider the full coupling between thermal, fluid flow and stress analysis of all the relevant materials, including casting, cores and dies. Some of the considerations to be addressed when translating this concept into a commercial code include appropriate material models, appropriate thermal/mechanical contact algorithms, hot tearing, cracking and die fatigue predictions, among others.Gap Formation
The main reasons for stress formation are mechanical resistance of the mould and nonhomogeneous temperature gradients. Therefore, the influence of an air gap formation or inversely contact pressures between the mould and the solidified casting must be taken into account. Indeed, this phenomenon also controls the heat transfer of the casting/mould interface and consequently greatly influences the above listed defects prediction. This requires a coupled thermal and stress analysis possible only with the FEM technique. For demonstration purposes, a simple T shaped casting of A356 in a H13 mould is simulated, as shown in Figure 1. The effective interface heat transfer coefficient at two different points on the casting is plotted in Figure 2. The top curve is from a point experiencing increasing contact pressure as the casting contracts. The middle curve is from a point where a gap is opening up between casting and mould, assuming the presence of air. The bottom curve is from that same point, but assuming a vacuum. The large variation in the coefficient illustrates the importance of accounting for local conditions by coupling thermal and mechanical calculations. In addition, this example illustrates the value of the reverse coupling of the mechanical deformations with the energy solution. This effect
can be seen in Figure 1 where the heat flux contours are plotted. The heat flux is greatest where the contact pressure is highest. This phenomenon will result in a different solidification path between a coupled and uncoupled calculation which could greatly influence the prediction of defects such as hot tearing as shown in Figure 3. Indeed, whether or not hot tearing occurs depends on the mechanical loads that develop due to thermal contraction and the contact constraints of the die wall.1.40000E+03
1.00000E+03 h _ e ff (W /m ^2 K )
Gap air Gap closed Gap vacuum
0.00000E+00 0 200 400 T ime (s) 600 800 1000
Figure 1: Heat Flux Contours influenced by the gap formations. (ProCAST)
Figure 2: Interface heat transfer coefficients taking into account the mechanical contact.
Figure 3: Hot tearing indicator showing different sensitivity and location between a coupled and uncoupled calculation. (ProCAST, Low Pressure Die Casting of Brass component, courtesy of KWC Engineering AG, Switzerland)
Industrial Example-Quality Map
ProCAST  provides a unique solution based on a fully coupled thermal, flow and stress model in order to have accurate prediction of hot tearing, cracking, part distortion as well as die distortion and die fatigue life. The first example concerns a low pressure die casting of an aluminium automotive wheel, courtesy of C.M.S. Jant Ve Makina San A.S. in Turkey. The plots in figure 4, showing residual stresses, hot tearing sensitivity and deformations, indicate where the integrity of the casting and the die is of particular importance thereby acting as a component Quality map to the foundry man.
Residual stresses in the casting
Shear stresses in the mould
Hot tearing prediction
Enlarged deformation observed during cooling Figure 4: Stress modelling. (ProCAST)
Industrial Example-Shape Prediction
The second example (see Figure 5) concerns a gravity shell casting of a stainless steel AISI 410 component, courtesy of Fundiciones en Cascara S.A., in Spain. One of the major issues in casting remains the deformation of the part with regards to the tight tolerances required by the industry. When a casting cools at room temperature, thermal stresses and dimensional changes occur. The dimensional changes depend on the casting's geometry, temperature and material properties. The scope of this calculation is to accurately predict the final shape of the component in order to make a reverse pattern of the shell to compensate the contraction and the deformation of the casting. This will help to approach the final shape of the part required by the customer specifications. Solidification and stress analysis were performed on the component by taking into account springback effect of the part after removing the material mould. To validate the simulation results, 3D digitalization of the real part was carried out with a SIDIO machine. This technique without contact allows getting a thousand of points representing the actual geometry with a precision of 0.1mm. Then, recomposed shape could be superimposed with CAD geometry as shown in figure 6 to see any shape differences. Simulation results showed good correlations with the final shape of the part in terms of tendencies and absolute displacements.
Simulated results (temperature field, ProCAST) Figure 5: Stainless steel shell casting component.
Figure 6: Comparison between the actual digitized geometry (red points or contours on the left) and computed results by ProCAST (red tetrahedral mesh on the right) and the original CAD/Mesh geometry in black or blue (on both sides) is shown.
ESI Group, editor of ProCAST and PAM-QUIKCAST products contributes to the IMPRESS1 project with the development of its simulation software on (i) coupling casting and heat treatment simulation, (ii) assessment of solid state transformations during heat treatment of TiAl intermetallic alloys, and (iii) prediction of material properties as a function of microstructures and porosity.
MICRO AND GAS POROSITY This section is a summary of the paper published by G. Couturier and M. Rappaz, Modeling of Porosity Formation in Multicomponent Alloys in the presence of several dissolved Gases and Volatile Solute Elements, Symposium on Simulation of Aluminum Shape Casting Processing, Edited by Qigui Wang (TMS, 2006).
The final integrity of a casting, e.g. mechanical properties and surface finish, is greatly influenced by the presence of porosity. In most of simulation software today, porosity prediction is limited to macro-shrinkage porosity which corresponds to the contraction of the metal during solidification. This approach does not take into account for gas and interdendritic shrinkage porosity. Gas porosity in aluminium alloy is due to the segregation of hydrogen dissolved in the molten metal as it has almost no solubility in the solid phase. Therefore, as shown in figure 7, porosity is the result of the combination of